Synthesis via RAFT Polymerization of Tadpole-Shaped Organic/Inorganic Hybrid Poly(acrylic acid) Containing Polyhedral Oligomeric Silsesquioxane (POSS) and Their Self-assembly in Water
Post on 16-Feb-2017
Embed Size (px)
Synthesis via RAFT Polymerization of Tadpole-Shaped Organic/Inorganic Hybrid Poly(acrylic acid) Containing Polyhedral OligomericSilsesquioxane (POSS) and Their Self-assembly in Water
Weian Zhang,, Bing Fang, Andreas Walther, and Axel H. E. Muller*,
Makromolekulare Chemie II, UniVersitat Bayreuth, D-95440 Bayreuth, Germany, and Laboratory forAdVanced Materials, Department of Chemistry, East China UniVersity of Science and Technology, 130Meilong Road, Shanghai 200237, P. R. China
ReceiVed December 16, 2008; ReVised Manuscript ReceiVed February 17, 2009
ABSTRACT: Tadpole-shaped inorganic/organic hybrid poly(tert-butyl acrylate) was prepared by RAFTpolymerization of tert-butyl acrylate (tBA) using a POSS-containing chain transfer agent (CTA). The polymerizationkinetics showed a pseudofirst-order behavior with a short induction period; the number-average molecular weightslinearly increase with conversion. In conjunction with low polydispersity (PDI < 1.3), this confirms a controlledpolymerization. POSS-PtBA was further hydrolyzed into amphiphilic, tadpole-shaped poly(acrylic acid) (POSS-PAA). The self-assembly behavior of POSS-PAA in aqueous solution at pH ) 8.5 was investigated by transmissionelectron microscopy (TEM) as well as static and dynamic light scattering (SLS and DLS). The results show thatPOSS-PAA self-assembles in water into rather large aggregates where the POSS moieties are dispersed in theparticle. The size (average radius 60 nm by DLS) is nearly independent of the chain length of PAA. Theaggregates are pH-responsive, contracting when decreasing pH from 8.5 to 4.
Organic-inorganic hybrid materials have attracted greatinterest in recent years, due to the combination of propertiesderived from the organic and inorganic components.1-5 Poly-hedral oligomeric silsesquioxanes (POSS), a class of uniqueinorganic components, can be incorporated into polymermatrices to produce many novel hybrid polymers with advanta-geous properities.6-9 POSS molecules have a cage-shaped three-dimensional structure with the formula (RSiO1.5)n, (n g 6).Among them, octasilsesquioxanes (R8Si8O12) (n ) 8) have beenmostly investigated; they consist of a rigid, cubic silica corewith a 0.53 nm side length, where each of the eight cornerscarries one organic group. The corner groups can be reactiveor unreactive groups, which provide the POSS molecules withthe higher reactivity and solubility in organic solvents.10-12
Thus, the POSS molecules are much more variable in theirproperties as compared to other inorganic components, suchclays or carbon nanotubes. POSS molecules can be incorporatedinto almost all kinds of the polymer matrices by blending,grafting, cross-linking or copolymerization, to produce POSS-containing organic-inorganic hybrids with many promisingproperties such as enhanced mechanical and thermal properties,oxidation resistance, and reduced flammability.6-9,13-28
In previous research, much attention has been focused on thepreparation methods and the properties of POSS-containinghybrid polymers. For example, atom-transfer radical polymer-ization (ATRP) has been used to prepare POSS-containinghybrid polymers with different topological structures such asstar-shaped, block and tadpole-shaped hybrid polymers.29-31
Telechelic and hemitelechelic POSS-containing hybrid polymerswere also synthesized by urethane formation between hydroxy-terminal polymers and isocyanate group of POSS mol-ecules.32-35 However, there are still many other novel aspectsworthy to be studied, especially the self-assembly behavior ofthese hybrid polymers with novel architectures. POSS molecules
were also used to modify polystyrene-block-polybutadiene-block-polystyrene (SBS) triblock copolymers and the bulkmorphology of the block copolymers was still preserved.36,37
Zhu et al. investigated the self-assembly and chain-folding inwell-defined oligomeric polyethylene-block-poly(ethylene oxide)-block-POSS (PE-b-PEO-b-POSS) triblock co-oligomers.38 Pyunand Matyjaszewski first reported the synthesis of ABA triblockcopolymers with a POSS-containing methacrylate monomer viaATRP, and the self-assembly structure formed in thin films.39,40
POSS-containing diblock copolymers were also prepared byanionic polymerization and lamellar bulk structures wereobserved.41 Recently, W. Zhang et al. synthesized tadpole-shaped hybrid poly(N-isopropylacrylamide) (PNIPAAm) usinga POSS-containing reversible addition-fragmentation transfer(RAFT) agent.42 The tadpole-shaped POSS-PNIPAAm self-assembles into core-shell nanostructured micelles with uniformdiameter.
In this contribution, we extend the study of the self-assemblyof POSS-containing hybrid polymers toward polyelectrolytes.We synthesized amphiphilic POSS-containing tadpole-shapedhybrid poly(acrylic acid) (PAA) using RAFT polymerizationof tert-butyl acrylate (tBA). The POSS-PAA was prepared viathe hydrolysis of POSS-PtBA using trifluoroacetic acid. Theself-assembly behavior of the hybrid POSS-PAA was investi-gated by transmission electron microscopy (TEM) and lightscattering (DLS and SLS).
Materials. Aminoisobutyl polyhedral oligomeric silsesquioxane(POSS) was purchased from Hybrid Plastics Company. tert-Butylacrylate (tBA) was kindly supplied by BASF SE, and was passedthrough an silica column to remove the inhibitor. Other regents inanalytical grade were all obtained from Aldrich. Azobisisobuty-ronitrile (AIBN) was recrystallized from ethanol. Dichloromethanewas dried over CaH2 and distilled before use. The RAFT agent,3-benzylsulfanylthiocarbonylsufanylpropionic acid (BSPA), wassynthesized according to the literature.43
3-Benzylsulfanylthiocarbonylsufanyl-N-(3-(isobutyl polyhedraloligomeric silsesquioxane) propyl)propanamide (POSS-BSPA). Thesynthesis of the POSS-containing RAFT agent, POSS-BSPA, was
* Corresponding author. E-mail: email@example.com. Makromolekulare Chemie II, Universitat Bayreuth. Laboratory for Advanced Materials, Department of Chemistry, East
China University of Science and Technology.
2563Macromolecules 2009, 42, 2563-2569
10.1021/ma802803d CCC: $40.75 2009 American Chemical SocietyPublished on Web 03/10/2009
reported in our previous paper.42 The resulting product was furthercrystallized in petroleum ether with a yield of 80%. 1H NMR(CDCl3, ppm): 7.27-7.34 (m, 5H, Ph), 4.61 (s, 2H, CH2Ph), 3.67(t, 2H, -Si-CH2CH2CH2NH-), 3.25 (q, 2H, -HNCOCH2CH2S-),2.60 (t, 2H, -HNCOCH2CH2S-), 1.85 (m, 7H, -Si-CH2CH(CH3)2), 1.60 (m, 2H, -Si-CH2CH2CH2NH-), 0.95 (d,42H, -Si-CH2CH(CH3)2), 0.60 (m, 16H, -Si-CH2CH(CH3)2,-Si-CH2CH2CH2NH-).
Synthesis of POSS-PtBA. A typical polymerization procedurefor the synthesis of POSS-containing inorganic/organic hybrid PtBAas follows: A round-bottom glass flask (50 mL) with a magneticstir bar was charged with tBA (3 mL, 20.67 mmol), POSS-containing RAFT agent (125.5 mg, 0.11 mmol), AIBN (6.08 mg,0.037 mmol) and 15 mL of toluene. The mixture solution waspurged with argon for 30 min, and then the glass tube was sealedunder argon. The polymerization was carried out in a thermostattedoil bath at 70 C. Small samples (about 0.5 mL) were taken outfrom the reaction flask at intervals to check the conversion, whichwas measured by 1H NMR by comparing the peaks of the doublebond protons of tBA at 5.75 ppm and of the toluene aromaticprotons at 7.23 ppm. At the end of the polymerization reaction,the polymerization was stopped by plunging the tube into ice water.The polymerization flask was opened, and then precipitated into250 mL cold mixed solution of methanol/water (3/1, v/v). Theprecipitate was redissolved in dioxane, and the product was driedby freeze-drying for two days. 1H NMR (dioxane-d8, ppm):7.15-7.23 (m, 5H, Ph), 2.10-2.35, 1.65-1.93 (m, polymerbackbone protons, -Si-CH2CH(CH3)2), 1.44 (s, -COO(CH3)3),0.97 (d, -Si-CH2CH(CH3)2)), 0.62 (m, -Si-CH2CH(CH3)2,-Si-CH2CH2CH2NH-). Mn(GPC) ) 15 870, Mw/Mn ) 1.20.
Preparation of POSS-PAA from POSS-PtBA. A typicalprocedure for the conversion of POSS-PtBA to POSS-PAA asfollows: a round-bottom flask (50 mL) with a magnetic stir barwas charged with POSS-PtBA60 (Mn ) 8, 374, 0.5 g, 3.4 mmol oftert-butyl acrylate unit) followed by dichloromethane (40 mL). Themixture was allowed to stir for 15 min to dissolve the polymer.And then trifluoroacetic acid (TFA; 4.0 mL, 53.0 mmol) was added.The mixture was allowed to stir at room temperature for 24 h. After24 h, a yellow precipitate had formed, and dichloromethane andTFA were removed by rotary evaporation. The product was washedthree times with dichloromethane, and then redissolved in dioxide,and followed by freeze-drying to afford the light yellow powder.
1H NMR (dioxane-d8, ppm): 7.15-7.23 (m, 5H, Ph), 2.20-2.53,1.37-1.93 (m, polymer backbone protons, -Si-CH2CH(CH3)2),0.97 (d, -Si-CH2CH(CH3)2)), 0.62 (m, -Si-CH2CH(CH3)2,-Si-CH2CH2CH2NH-)).Mn)4,953,Mw/Mn)1.10(MALDI-TOF).
Self-assembly of POSS-PAA in Aqueous Solution. A typicalself-assembly aggregate solution was prepared as following: POSS-PAA60 (100 mg) was first dissolved in dioxane (25 mL), which isa good solvent for POSS-PAA. The solution was stirred overnight,and gradually dialyzed against pH 8.5 Millipore water (resistance) 18 M) for 3 days. After gradual dialysis, the self-assemblyaggregate solution was dialyzed at least three times using pH 8.5Millipore water to make sure to completely remove dioxane.
Nuclear Magnetic Resonance Spectroscopy (NMR). The1H NMR and 13C NMR measurements were carried out on aBruker AC-250 instrument. The samples were dissolved indeuterated CDCl3 and dioxane-d8, respectively, and the solutionswere measured with tetramethylsilane (TMS) as an internalreference. By comparing the peaks of the polymer backbonemethine protons at 2.22 ppm and the tert-butyl protons at 1.45ppm with the methyl protons of the hepta(isobutyl) groups ofPOSS at 0.97 pm, the number-average degrees of polymerizationand the corresponding molecular weights were determined asMn,NMR ) [((I1.45/9) + I2.22)/2]/[I0.97/42] MtBA + MCTA., where,MtBA and MCTA are the molecular weights of monomer and CTA,respectively. 29Si NMR spectra were measured on a Varian Inova300 MHz spectrometer at 23 C. The samples were dissolved
in dioxane-d8; chemical shifts are given relative to TMS [29Si) 0 ppm for (29Si) ) 19.867184 MHz]; Chemical shifts aregiven to ( 0.1 for 29Si; coupling constants are given ( 0.4 Hzfor J(29Si). The spectra were measured by using the refocusedINEPT pulse sequence based on 2/3J(29Si) ) 10 Hz afteroptimizing the delay times in the pulse sequence.
Fourier Transform Infrared Spectroscopy (FTIR). Mea-surements were conducted on a Bruker Equinox 55/s Fouriertransform spectrometer at room temperature (25 C). Thesamples mixed with KBr were granulated into powder andpressed into flakes for IR measurements.
Gel Permeation Chromatography (GPC). The molecularweights and molecular weight distribution were measured byconventional GPC. Column set: 5 m SDV gel, 102, 103, 104,and 105 , 30 cm each (PSS, Mainz). Detectors used are RIand UV operated at 254 nm. Polystyrene standards (PSS, Mainz)with narrow molecular weight distribution were used for thecalibration of the column set, and tetrahydrofuran (THF) wasused as the eluent at a flow rate of 1 mL/min. Since thecalibration curve of PtBA is different from that of PS, we usedthe number-average molecular weights obtained from the NMRsignals of POSS and PtBA.
MALDI-TOF Mass Spectrometry. MALDI-TOF massspectrometry was performed on a Bruker Reflex III instrumentequipped with a 337 nm N2 laser in the reflector mode and 20kV acceleration voltage. 2,5-Dihydroxybenzoic acid (Aldrich,97%) was used as a matrix. Samples were prepared from THFsolution by mixing matrix (20 mg/mL) and polymer (10 mg/mL) in a ratio of 4:1. The number-average molecular weightsof the polymers were determined in the linear mode.
Transmission Electron Microscopy (TEM) images weretaken out on a Philips CM 20 TEM operated at 200 kV. A5 L droplet of self-assembly aggregate solution (0.5 mg/mL)was directly dropped onto a copper grid (300 mesh) coated witha carbon film, followed by drying at room temperature.
Cryogenic Transmission Electron Microscopy (cryo-TEM).The sample was prepared as described above. To achieve thedesired ionic strength, CsCl (Acros) was used. A drop of thesample (concentration around 4.0 mg/mL) was directly put ona lacey grid, where most of the liquid was removed with blottingpaper, leaving a thin film stretched over the lace. The specimenswere instantly shock vitrified by rapid immersion into liquidethane and cooled to approximately 90 K by liquid nitrogen ina temperature-controlled freezing unit (Zeiss Cryobox, ZeissNTS GmbH, Oberkochen, Germany). The temperature wasmonitored and kept constant in the chamber during all thesample preparation steps. After the sample is frozen, it wasinserted into a cryo-transfer holder (CT3500, Gatan, Munchen,Germany) and transferred to a Zeiss EM922 EFTEM. Examina-tions were carried out at temperatures around 90 K at anacceleration voltage of 200 kV. Zero-loss filtered images (E) 0 eV) were taken under reduced dose conditions (100-1000electrons/nm2). All images were registered digitally by a bottom-mounted CCD camera system (Ultrascan 1000, Gatan) combinedand processed with a digital imaging processing system (GatanDigital Micrograph 3.10 for GMS 1.5).
Dynamic Light Scattering (DLS) was carried out on an ALVDLS/SLS-SP 5022F compact goniometer system with an ALV5000/E correlator and a He-Ne laser ( ) 632.8 nm). Beforethe light scattering measurements, the sample solutions werefiltered three times by using Millipore Teflon (Nylon) filterswith a pore size of 0.45 m. A CONTIN analysis was takenfor the measured intensity correlation functions. Apparenthydrodynamic radii, Rh, of the self-assembly aggregates werecalculated according to the Stokes-Einstein equation. Allmeasurements were carried out at room temperature. The
2564 Zhang et al. Macromolecules, Vol. 42, No. 7, 2009
measurements were performed at fixed scattering angle of 90.The polymer solutions had a concentration of 2 mg/mL.
Static Light Scattering (SLS) was measured on a Soficagoniometer using a He-Ne laser ( ) 632.8 nm). Prior to thelight scattering measurements, the sample solutions were filteredthree times by using Millipore Teflon (Nylon) filters with a poresize of 0.45 m. Five concentrations of the polymer in aqueoussolution were measured at angles in the range from 30 to 150.Weight-average molecular weights, Mw, of the self-assemblyaggregates were obtained by the analysis of the Zimm plots.The refractive index increment of the POSS-PAA aggregatesin aqueous solution at 25 C was measured using a PSS DnDc-2010/620 differential refractometer, and the dn/dc of POSS-PAA35 and POSS-PAA60 are 0.1065 and 0.1119 mL/g, respec-tively.
Results and Discussion
RAFT Polymerization of tBA Using a POSS-ContainingRAFT Agent. The detailed description of the synthesis of thePOSS-containing RAFT was reported in...